Perovskite solar cells employing organic
, Aswani Yella2
, Yong Hui Lee2
, Guillermo Mı´nguez Espallargas1
, Michael Graetzel2
Mohammad K. Nazeeruddin2
and Henk J. Bolink1
*Thin-ﬁlm photovoltaics play an important role in the quest for clean renewable energy. Recently, methylammonium lead halide perovskites were identiﬁed as promising absorbers for solar cells1. In the three years since, the performance of perov-skite-based solar cells has improved rapidly to reach efﬁciencies as high as 15%1–10. To date, all high-efﬁciency perovskite solar cells reported make use of a (mesoscopic) metal oxide, such as Al2O3, TiO2or ZrO2, which requires a high-temperature sin-tering process. Here, we show that methylammonium lead iodide perovskite layers, when sandwiched between two thin organic charge-transporting layers, also lead to solar cells with high power-conversion efﬁciencies (12%). To ensure a high purity, the perovskite layers were prepared by sublimation in a high-vacuum chamber. This simple planar device structure and the room-temperature deposition processes are suitable for many conducting substrates, including plastic and textiles.
The hybrid organic–inorganic methylammonium lead halide perovskites, pioneered by Mitzi, are recognized for their excellent semiconducting properties11,12. Following the pioneering work of Miyasaka and co-workers1, the ease with which these organic–inor-ganic hybrid perovskite materials can be prepared and processed from solution makes them attractive for photovoltaic applications13. In their studies, the methylammonium lead iodide perovskite was used as a sensitizer in liquid dye-sensitized solar cells and an efﬁ-ciency of 3.8% was obtained. The low efﬁefﬁ-ciency results from the solubility of the perovskite layer in the iodine/iodide redox electro-lyte system. High efﬁciencies have been realized by replacing the liquid electrolyte with a solid hole-transporting material such as 2,2′,7,7′-tetrakis(N,N-di-p-methoxyphenylamine)-9,9′ -spirobiﬂuor-ene (spiro-MeOTAD), as reported by the groups of Snaith and Graetzel2–9. Interestingly, Lee et al.6 showed that a mixed-halide perovskite on a mesoporous Al2O3 photoanode acts both as a light absorber and an electron conductor. Etgar et al.8 reported that the pure methylammonium lead iodide perovskite also acts as an efﬁcient hole conductor. Recently, Burschka et al.4published a high power-conversion efﬁciency of 15% for a solar cell in which the perovskite was deposited by a novel sequential deposition technique on a mesoporous TiO2 ﬁlm. Ball et al.5showed that a thick layer (350 nm) of the mixed-halide methylammonium lead perovskite (CH3NH3PbI32xClx) leads to efﬁcient solar cells (12%). They argue that the perovskite functions as the absorber and as the electron and hole transporter. Additionally, it was suggested that the excitons dissociate predominantly in the bulk and not at a donor–acceptor interface. The operating mechanism of planar perovskite solar cells, however, is not clear. For example, it was shown that the photoluminescence of a mixed-halide methylammonium lead perovskite was reduced strongly when either a hole- or an electron-transporting layer was deposited on
top of it14. A similar effect, but less strong, was observed for thin ﬁlms of the pure iodide methylammonium lead perovskite14. Hence, exciton dissociation may occur both in the bulk and at the perovskite interface. Currently, the dominant process is not established and may well depend on the exact nature of the perovskite ﬁlm. Up to now, the highest efﬁciency was reported by Liu et al., who used a thin metal oxide layer and a sublimed perovskite layer that leads to solar cells with an efﬁciency of 15.4%9. High material purity is essential for efﬁcient charge-carrier transport and to prevent exciton quenching, as established in organic light-emitting diodes and organic photovoltaic (OPV) devices15,16. Therefore, in these devices vacuum sublimation is employed frequently to achieve high-purity layers. Solution-processed perovskites are generated in situ and therefore may contain imperfections and impurities. Puriﬁcation of the perovskite layer is not possible as it decomposes on dissolving.
An inverted layout, similar to that employed in small molecular weight and polymeric solar cells, has also been described17,18. In these bilayer planar heterojunction devices, the perovskite layer was used as the electron donor in combination with an electron acceptor, in analogy to a frequently used OPV layout. The holes are extracted via the transparent conductor poly(3,4-ethylenedioxy-thiophene):poly(styrenesulfonic acid) (PEDOT:PSS). The device performances, however, were signiﬁcantly inferior to those of devices that employ (mesoporous) metal oxides.
Here, we present an inverted thin-ﬁlm solar cell based on a sub-limed methylammonium lead iodide perovskite layer sandwiched between two very thin electron- and hole-blocking layers that consist of organic molecules. The organic materials were deposited using solution-based processes, whereas the CH3NH3PbI3 perov-skite and the metal contact were deposited using thermal evapor-ation under vacuum. These simple devices, free of metal oxide and prepared using room-temperature processing, reach efﬁciencies as high as 12% at 100 mW cm22, which demonstrate their potential for a wide variety of photovoltaic applications.
The CH3NH3PbI3perovskite thin ﬁlm was prepared by coeva-poration of the two starting compounds, CH3NH3I and PbI2. Details of the experimental conditions are given in the Methods section. These ﬁlms were characterized using grazing incidence X-ray diffraction (GIXRD). Initially, excess PbI2 was present in the ﬁlm, yet on optimizing the evaporation process, highly oriented pure CH3NH3PbI3 ﬁlms were obtained (see Fig 1a and Supplementary Fig. 1). The ﬁlms adopt the typical tetragonal struc-ture for CH3NH3MX3hybrid perovskites (M ¼ Pb, Sn; X ¼ Cl, Br, I) formed by a three-dimensional anionic framework of PbI6 octahe-dra with the methylammonium cations in the interstitial space (see Fig. 1b)19. The roughness of the CH
3NH3PbI3ﬁlm was evaluated using atomic force microscopy (AFM) and an image of a typical
Instituto de Ciencia Molecular, Universidad de Valencia, C/Catedra´tico J. Beltra´n 2, 46980 Paterna (Valencia), Spain,2
Laboratory of Photonics and Interfaces, Swiss Federal Institute of Technology (EPFL), Station 6, Lausanne, CH 1015, Switzerland.*e-mail: mdkhaja.nazeeruddin@epﬂ.ch; email@example.com
PUBLISHED ONLINE: 22 DECEMBER 2013 |DOI: 10.1038/NPHOTON.2013.341
scan is given in Fig. 1d, which demonstrates a smooth ﬁlm with a root mean square roughness of 5 nm. Figure 1c is a photograph of a 20-nm-thick ﬁlm.
As the CH3NH3PbI3layer is prepared via vacuum sublimation, it can be implemented easily in different device architectures. To demonstrate that the CH3NH3PbI3is capable of performing most of the roles required to obtain an efﬁcient solar cell and to minimize the use of costly organic semiconductors, a simple device structure was chosen. In this structure, which is typical for both organic photovoltaic and light-emitting devices, a semitransparent organic conductor was used as the positive charge-collecting contact. The structure of the device is shown in Fig. 2a, and consists of a 70 nm PEDOT:PSS layer and a thin layer (,10 nm) of poly(N,N′-bis(4-butylphenyl)-N,N′-bis(phenyl)benzidine) (polyTPD) (Fig. 2c) as the electron-blocking layer. On top of this, the CH3NH3PbI3was evaporated thermally to a thickness of 285 nm followed by a thin layer (,10 nm) of (6,6)-phenyl C61-butyric acid methyl ester (PCBM) as the hole-blocking layer (Fig. 2d)20. The device was completed by the evaporation of an Au top electrode (100 nm). Both the polyTPD and the PCBM layers were deposited using a meniscus-coating process to ensure high-quality ﬁlms21. The thickness of the layers was established using absorbance measurements.
The relevant energy levels of the materials used to prepare the solar cell are depicted in Fig. 2b. The valence band (VB) and
conduction band (CB) of the CH3NH3PbI3 perovskite are 25.4 and 23.9 eV, versus vacuum, respectively7. On illuminating the device, excitons are generated in the CH3NH3PbI3perovskite layer. It was reported that excitons in CH3NH3PbI3 perovskites are of the Wannier–Mott type, which implies that they may dissociate in the bulk of the perovskite layer5,12. Owing to the use of indium–tin oxide (ITO)/PEDOT:PSS as the hole-collecting contact and Au as the electron-collecting electrode, the built-in voltage of this device is small. Hence, to direct the ﬂow of electrons and holes, thin hole-blocking and electron-blocking layers are incorporated adjacent to the perovskite layer. PolyTPD and PCBM were selected for this role as their highest occupied molecular orbital (HOMO) and lowest unoccupied molecular orbital (LUMO) levels, respectively, match well with the VB and CB of the perovskite, which allows for a good transport of holes towards the polyTPD and of electrons to the PCBM layer (Fig. 2b). As the LUMO of polyTPD is signiﬁcantly closer to vacuum compared with that of the perovskite CB, polyTPD efﬁciently blocks the ﬂow of electrons. The opposite process, the blocking of holes, occurs at the perovskite–PCBM interface because of the lower HOMO of PCBM compared with that of the perovskite VB. As mentioned above, exciton dissociation may also occur at the perovskite–polyTPD and perovskite–PCBM interfaces14. Figure 3a shows the current–voltage (J–V) characteristics of a typical small-area (0.09 cm2) perovskite solar cell measured in the dark and under light intensities of 100, 50 and 10 mW cm22. The 0.0 0 5 10 15 20 25 0.5 1.0 1.5 2.0 2.5 3.0 Z (nm) X (µm) 10 10 10,000 20,000 30,000 40,000 50,000 60,000 70,000 80,000 15 20 25 30 35 40 45 50 2θ (°) Experimental ITO Simulated 840 nm a b d c
Figure 1 | Characteristics of the sublimed CH3NH3PbI3perovskite layer. a, GIXRD pattern with Cu Ka1radiation (l¼ 1.54056 Å) of the sublimed thin ﬁlm
(blue), ITO substrate (red) and calculated for CH3NH3PbI3with preferred orientation along the (100) and (001) directions.b, Simulation of the crystal
structure of CH3NH3PbI3perovskite. Pb atoms are placed at the centre of the grey octahedrons, lavender spheres represent iodine atoms and green spheres
represent the methylammonium cations.c, Photograph of a 20-nm-thick ﬁlm. d, AFM image and proﬁle of a 60-nm-thick ﬁlm.
reproducibility from device to device was excellent, with less than 10% deviation. The short-circuit current density (JSC), open-circuit voltage (VOC) and ﬁll factor (FF), respectively, are 16.12 mA cm22, 1.05 V and 0.67, which lead to a power-conversion efﬁciency of 12.04% measured at 100 mW cm22. At 50 and 10 mW cm22the device exhibited very similar efﬁciencies, 12.04% and 12.00%, respectively. The high open-circuit potential indicates that there are negligible surface and sub-bandgap states in the perovskite ﬁlm. The device performance under 100 mW cm22 is remarkable in view of the very thin perovskite ﬁlm of 285 nm. A device with cells of larger area (0.98 cm2) was also prepared and evaluated at 100 mW cm22 (Supplementary Fig. 4). The JSC and VOCare very similar to the data obtained for the small-area cell (14.76 mA cm22and 1.05 V, respectively). The FF, however, is sig-niﬁcantly lower (0.52), which is the main reason for the lower power-conversion efﬁciency (8.27%) for these larger cells.
The incident photon-to-current conversion efﬁciency (IPCE) spectra exhibit 74% (Fig. 3b) where the generation of photocurrent started at 790 nm, in agreement with the bandgap of the CH3NH3PbI3. It is interesting that the IPCE spectra show a very steep onset, contrary to the IPCE spectra reported for TiO2 and Al2O3mesoscopic-based perovskite cells. A very similar IPCE spec-trum as observed for our solar cells was reported for a solar cell based on a perovskite layer sandwiched between a C60-modiﬁed TiO2layer and a layer of poly(3-hexylthiophene)22. As such, the steep onset may be related to the speciﬁc interaction of the perov-skite with the fullerene molecules. The IPCE spectrum is almost ﬂat, except for a dip at 630 nm that could result from the oxidized polyTPD acting as a ﬁlter or from reduced absorption of the perov-skite. Integrating the overlap of the IPCE spectrum with the AM1.5G solar photon ﬂux yields a current density of 16.40 mA cm22, which is in excellent agreement with the measured photocurrent density of N Au Vacuum Ener gy ITO PCBM PCBM PolyTPD P olyTPD PEDOT:PSS PEDO T :PS S ITO N n O OCH3 CH3NH3Pbl3 (100 nm) (10 nm) (10 nm) (70 nm) (285 nm) CH3NH3Pbl3 −2.4 −3.9 a b c d Au −3.9 −4.8 −5.3 −5.4 −5.4 −5.9 −5.4
Figure 2 | Schematics of the device. a, Stacked layer structure. b, Schematic of the relative energy levels of each layer. c, Chemical structure of the polyarylamine (polyTPD).d, Chemical structure of PCBM.
3 2 1 0 100 80 60 40 20 0 400 500 600 700 800 Wavelength (nm) Voltage (V) C urr ent densit y (mA cm −2 ) Absorbanc e IPCE (%) 94.6% sun 49.5% sun 9.3% sun Dark 0 0.0 0.2 0.4 0.6 0.8 1.0 1.2 2 4 6 8 10 12 14 16 18 20 a b
Figure 3 | Typical J–V and IPCE characteristics of the perovskite solar cell. a, Photocurrent density versus voltage at 100, 50 and 10 mW cm22and in the dark.b, IPCE spectrum and absorbance of a 285-nm-thick perovskite layer.
NATURE PHOTONICSDOI: 10.1038/NPHOTON.2013.341
16.12 mA cm22 at the standard solar AM1.5G intensity of 100 mW cm22, which conﬁrms that the mismatch between the simulated sunlight and the AM1.5G standard is negligible. The absorbance of the CH3NH3PbI3ﬁlm is similar to those reported previously for this material and increases with increasing layer thickness (Fig. 3b). The absorption extends over the complete visible spectrum up to 800 nm, with a local maximum around 500 nm (the scale of the graph in Fig. 3b is optical density).
An efﬁcient solid-state, thin-ﬁlm solar cell was obtained by sand-wiching a sublimated CH3NH3PbI3 perovskite layer between two thin organic charge-transporting layers that function as hole and electron blockers, respectively, and contacting it via an indium tin oxide (ITO)/PEDOT:PSS as the hole-extraction and an Au electroextraction contact. The simple device architecture, which is an n-type oxide and scaffold free, coupled with easy room-temperature fabrication using economically favourable materials, high efﬁciency and high reproducibility rivals strongly the established thin-ﬁlm photovoltaic technologies. The device power-conversion efﬁciency of 12% at 100 mW cm22 is remarkable in view of the very thin (285 nm) perovskite ﬁlm. The high Jscof 16.12 mA cm
22 and the open-circuit potential of 1.05 V reveal that very few electrons and holes recombine, which demonstrates the effectiveness of the hole- and electron-blocking layers. We believe that this new class of perovskite solar cell using organic semiconductors to collect the charges will ﬁnd widespread applications to rival photovoltaic solar cells based on thin ﬁlms.
Note added in proof: During the revision of this paper, a highly rele-vant article to this topic was published: P. Docampo, J.M. Ball, M. Darwich, G.E. Eperon & H.J. Snaith, Efﬁcient organometal trihalide perovskite planar-heterojunction solar cells on ﬂexible polymer substrates. Nature Commun. 4, 2761 (2013).
Materials.Photolithographically patterned ITO-covered glass substrates were purchased from NaranjoSubstrates. Aqueous dispersions of PEDOT:PSS (Clevios P VP Al 4083) were obtained from Heraeus Holding and used as received. Poly-TPD was purchased from ADS Dyesource. PbI2was purchased from Aldrich and used as
is. CH3NH3I was prepared similarly to a previously published method8; in brief,
CH3NH3I was synthesized by reacting 21.6 ml methylamine (40 wt% in water;
Aldrich) and 30 ml hydroiodic acid (57 wt% in water; Aldrich) in a 250 ml round-bottomed ﬂask at 0 8C for 2 h with stirring. The white precipitate was recovered by evaporation at 50 8C for 1 h. The product, CH3NH3I, was dissolved in ethanol,
ﬁltered, recrystallized from diethyl ether and dried at 60 8C in a vacuum oven for 24 h. Device preparation.Devices were prepared on cleaned ITO substrates by spin coating a thin layer of PEDOT:PSS from the commercial aqueous dispersion (1,200 revolutions per minute for 30 s (Chemmat, 3 cm diameter), which resulted in a thickness of 70 nm). On top of this layer a thin ﬁlm of polyTPD was deposited from a chlorobenzene solution (10 mg ml21) using a meniscus coater and a coating speed
of 2.5 mm s21. Then the substrates were transferred to a vacuum chamber integrated
into an inert glovebox (,0.1 ppm O2and ,0.1 ppm H2O; MBraun) and evacuated
to a pressure of 1× 1026mbar. Two ceramic crucibles were ﬁlled with CH 3NH3I
(freshly prepared) and PbI2, which were heated to 70 8C and 250 8C, respectively.
The ﬁlm thickness was controlled by the PbI2evaporation at a rate of evaporation of
0.5 Å s21(see Supplementary Information for more details concerning the
perovskite evaporation process). The PCBM layer was deposited using a chlorobenzene solution (10 mg ml21) in ambient conditions with a meniscus coater and a coating speed of 10 mm s21. The device was completed by the thermal evaporation of the top metal electrode under a base pressure of 2× 1026mbar to a thickness of 100 nm. The solar cells (active area of 0.09 and 0.98 cm2) were then encapsulated with a glass cover using an ultraviolet-curable epoxy sealant (Ossila E131 Encapsulation Epoxy), with an ultraviolet exposure of 5 min.
Characterization.GIXRD data were collected at room temperature in the 2u range 5–508 on an Empyrean PANalytical powder diffractometer using Cu Ka1radiation.
Typically, four repeated measurements were collected and merged into a single diffractogram. Pawley reﬁnements23were performed using the TOPAS computer
program24and revealed an excellent ﬁt to a one-phase model with a tetragonal cell
(a ¼ 8.80(2), c ¼ 12.57(2) Å) and space group I4/mcm. Additional peaks that correspond to the ITO substrate were also observed. The observed and
calculated diffraction patterns for the reﬁned crystal structures are shown in Supplementary Fig. 3.
Simulation of the crystal structure of CH3NH3PbI3perovskite was performed
using, as a starting model, the isostructural Sn analogue (CCDC ref. code: ZZZBWS02), and modifying the cell parameters to those obtained in the Pawley reﬁnement25.
Absorption spectra were taken using a ﬁbre-optics based Aventes Avaspec2048 spectrometer.
Current–voltage characteristics were recorded by applying an external potential bias to the cell and recording the generated photocurrent with a digital source meter (Keithley Model 2400). The light source was a 450 W xenon lamp (Oriel) equipped with a Schott K113 Tempax sunlight ﬁlter (Praezisions Glas & Optik) to match the emission spectrum of the lamp to the AM1.5G standard. A black mask was used in the photovoltaic studies to limit the active area of the device. Before each measurement, the exact light intensity was determined using a calibrated Si reference diode equipped with an infrared cut-off ﬁlter (KG-3, Schott). IPCE measurements were determined using a 300 W xenon light source (ILC Technology). A Gemini-180 double monochromator (Jobin Yvon) was used to select and increment the wavelength of the radiation that impinged on the cells. The monochromatic incident light was passed through a chopper run at 1 Hz frequency, and the on/off ratio was measured by an operational ampliﬁer. IPCE spectra were recorded as functions of wavelength under a constant white-light bias of approximately 5 mW cm22supplied
by an array of diodes that emitted white light. The excitation beam from a 300 W xenon lamp (ILC Technology) was focused through a Gemini-180 double monochromator (Jobin Yvon) and chopped at approximately 2 Hz. The signal was recorded using a Model SR830 DSP Lock-In Ampliﬁer (Stanford Research Systems).
Received 16 September 2013; accepted 14 November 2013; published online 22 December 2013
1. Kojima, A., Teshima, K., Shirai, Y. & Miyasaka, T. Organometal halide perovskites as visible-light sensitizers for photovoltaic cells. J. Am. Chem. Soc. 131,6050–6051 (2009).
2. Kim, H.-S. et al. High efﬁciency solid-state sensitized solar cell-based on submicrometer rutile TiO2nanorod and CH3NH3PbI3perovskite sensitizer.
Nano Lett. 13, 2412–2417 (2013).
3. Heo, J. H. et al. Efﬁcient inorganic–organic hybrid heterojunction solar cells containing perovskite compound and polymeric hole conductors. Nature Photon. 7, 486–491 (2013).
4. Burschka, J. et al. Sequential deposition as a route to high-performance perovskite-sensitized solar cells. Nature 499, 316–319 (2013).
5. Ball, J. M., Lee, M. M., Hey, A. & Snaith, H. J. Low-temperature processed meso-superstructured to thin-ﬁlm perovskite solar cells. Energy Environ. Sci. 6, 1739–1743 (2013).
6. Lee, M. M., Teuscher, J., Miyasaka, T., Murakami, T. N. & Snaith, H. J. Efﬁcient hybrid solar cells based on meso-superstructured organometal halide perovskites. Science 338, 643–647 (2012).
7. Kim, H-S. et al. Lead iodide perovskite sensitized all-solid-state submicron thin ﬁlm mesoscopic solar cell with efﬁciency exceeding 9%. Sci. Rep. 2, 591 (2012). 8. Etgar, L. et al. Mesoscopic CH3NH3PbI3/TiO2heterojunction solar cells. J. Am.
Chem. Soc. 134, 17396–17399 (2012).
9. Liu, M., Johnston, M. B. & Snaith, H. J. Efﬁcient planar heterojunction perovskite solar cells by vapour deposition. Nature 501, 395–398 (2013). 10. Hodes, G. Perovskite-based solar cells. Science 342, 317–318 (2013). 11. Kagan, C. R., Mitzi, D. B. & Dimitrakopoulos, C. D. Organic–inorganic hybrid
materials as semiconducting channels in thin-ﬁlm ﬁeld-effect transistors. Science 286,945–947 (1999).
12. Tanaka, K. et al. Comparative study on the excitons in lead-halide-based perovskite-type crystals CH3NH3PbBr3and CH3NH3PbI3. Solid State Commun.
13. Snaith, H. J. Perovskites: the emergence of a new era for low-cost, high-efﬁciency solar cells. J. Phys. Chem. Lett. 4, 3623–3630 (2013).
14. Stranks, S. D. et al. Electron-hole diffusion lengths exceeding 1 micrometer in an organometal trihalide perovskite absorber. Science 342, 341–344 (2013). 15. Sasabe, H. & Kido, J. Development of high performance OLEDs for general
lighting. J. Mater. Chem. C 1, 1699–1707 (2013).
16. Riede, M., Mueller, T., Tress, W., Schueppel, R. & Leo, K. Small-molecule solar cells—status and perspectives. Nanotechnology 19, 424001 (2008).
17. Jeng, J-Y. et al. CH3NH3PbI3perovskite/fullerene planar-heterojunction hybrid
solar cells. Adv. Mater. 25, 3727–3732 (2013).
18. Sun, S. et al. The origin of high efﬁciency in low-temperature solution-processable bilayer organometal halide hybrid solar cells. Energy Environ. Sci. http://dx.doi.org/10.1039/C3EE43161D (2014).
19. Mitzi, D. B. in Progress in Inorganic Chemistry, Vol. 48 (ed. Karin, K.D.) 1–121 (John Wiley, 2007).
20. Yu, G., Gao, J., Hummelen, J. C., Wudl, F. & Heeger, A. J. Polymer photovoltaic cells: enhanced efﬁciencies via a network of internal donor–acceptor heterojunctions. Science 270, 1789–1791 (1995).
21. Malinkiewicz, O., Lenes, M., Brine, H. & Bolink, H. J. Meniscus coated high open-circuit voltage bi-layer solar cells. RSC Adv. 2, 3335–3339 (2012). 22. Abrusci, A. et al. High-performance perovskite–polymer hybrid solar cells
via electronic coupling with fullerene monolayers. Nano Lett. 13, 3124–3128 (2013).
23. Pawley, G. S. Unit-cell reﬁnement from powder diffraction scans. J. Appl. Cryst. 14,357–361 (1981).
24. TOPAS-Academic, Version 4.1, 2007, http://www.topas-academic.net (Coelho Software, Brisbane).
25. Takahashi, Y. et al. Charge-transport in tin-iodide perovskite CH3NH3SnI3:
origin of high conductivity. Dalton Trans. 40, 5563–5568 (2011).
We thank A. Soriano-Portillo, J. Ferrando, A. K. Chandiran and E. Ortı´ for their assistance with the sample preparation and characterization, and careful proofreading of the manuscript. This work was supported by the European Community’s Seventh Framework Programme (ORION, Grant 229036 and NANOMATCELL, Grant 308997), the Spanish Ministry of Economy and Competitiveness (MAT2011-24594), the Generalitat Valenciana
(Prometeo/2012/053) and the Global Research Laboratory Program, Korea (GLOBASOL, Grant 309194).
O.M. designed, prepared and characterized the devices, A.Y. and Y.H.L. characterized the devices, G.M.E. supervised the X-ray characterization and interpretation, M.G. supervised the work and wrote the manuscript, M.K.N. initiated the research, provided key materials and wrote the manuscript, H.J.B initiated the research, designed the devices, supervised the work and wrote the manuscript.
Supplementary information is available in the online version of the paper. Reprints and permissions information is available online at www.nature.com/reprints. Correspondence and requests for materials should be addressed to M.K.N. and H.J.B.